J. Funct. Biomater. 2012, 3, 173-182; doi:10.3390/jfb3010173
ISSN 2079-4983 www.mdpi.com/journal/jfb/
Gas-Foamed Scaffold Gradients for Combinatorial Screening in 3D
Kaushik Chatterjee 1,2, Alison M. Kraigsley 1, Durgadas Bolikal 3, Joachim Kohn 3 and Carl G. Simon Jr. 1,*
1 Polymers Division, National Institute of Standards & Technology, 100 Bureau Drive, Gaithersburg, MD 20899, USA; E-Mail: firstname.lastname@example.org
2 Department of Materials Engineering, Indian Institute of Science, Bangalore 560012, India; E-Mail: email@example.com
3 New Jersey Center for Biomaterials, Rutgers University, Piscataway, NJ 08854, USA; E-Mails: firstname.lastname@example.org (D.B.); email@example.com (J.K.)
* Author to whom correspondence should be addressed; E-Mail: firstname.lastname@example.org; Tel.: +1-301-975-8574; Fax: +1-301-975-4977.
Received: 6 February 2012; in revised form: 28 February 2012 / Accepted: 1 March 2012 / Published: 7 March 2012
Abstract: Current methods for screening cell-material interactions typically utilize a two-dimensional (2D) culture format where cells are cultured on flat surfaces. However, there is a need for combinatorial and high-throughput screening methods to systematically screen cell-biomaterial interactions in three-dimensional (3D) tissue scaffolds for tissue engineering. Previously, we developed a two-syringe pump approach for making 3D scaffold gradients for use in combinatorial screening of salt-leached scaffolds. Herein, we demonstrate that the two-syringe pump approach can also be used to create scaffold gradients using a gas-foaming approach. Macroporous foams prepared by a gas-foaming technique are commonly used for fabrication of tissue engineering scaffolds due to their high interconnectivity and good mechanical properties. Gas-foamed scaffold gradient libraries were fabricated from two biodegradable tyrosine-derived polycarbonates: poly(desaminotyrosyl-tyrosine ethyl ester carbonate) (pDTEc) and poly(desaminotyrosyl-tyrosine octyl ester carbonate) (pDTOc). The composition of the libraries was assessed with Fourier transform infrared spectroscopy (FTIR) and showed that pDTEc/pDTOc gas-foamed scaffold gradients could be repeatably fabricated. Scanning electron microscopy showed that scaffold morphology was similar between the pDTEc-rich ends
J. Funct. Biomater. 2012, 3
and the pDTOc-rich ends of the gradient. These results introduce a method for fabricating gas-foamed polymer scaffold gradients that can be used for combinatorial screening of cell-material interactions in 3D.
Keywords: combinatorial screening; polymer; scaffold; tissue engineering
Combinatorial and high-throughput technologies are being applied for discovery in tissue engineering research to systematically screen cell-biomaterial interactions [1,2]. In current methods, material surfaces are prepared either as a continuous gradient or an array library where a property of the biomaterial is systematically varied . Cells are seeded on the biomaterial libraries and optimal properties are determined through measurement of the desired cellular responses. For example, cell response to polymer blends was measured using gradient scaffolds prepared from poly(-caprolactone) (PCL) and poly(D,L)lactic acid (PDLLA) to identify an optimal composition for osteoblast proliferation and differentiation . A large library of photopolymerized materials was screened using high-throughput technology to identify optimal substrates to support human embryonic stem cells in feeder-free conditions . Orthogonal gradients in surface wettability and topography were fabricated to screen osteoblast response to biomaterial surface properties . A combination of array and gradient approaches was applied to screen cell response to composition of dental composites . In another study, topochips were designed to rapidly screen the effect of surface topography on mesenchymal stem cell proliferation and differentiation .
However, in tissue engineering, biomaterials are commonly processed into three-dimensional (3D) scaffold for tissue regeneration . Cells are sensitive to topographical differences between 2D surfaces and 3D scaffolds [9,10] and studies indicate that cell response in 3D scaffolds is more representative of in vivo behavior than that observed in a 2D culture format . Thus, there is a need to design combinatorial techniques to screen 3D tissue scaffolds. A few recent studies have utilized combinatorial 3D tissue scaffolds . For example, gradient hydrogels were fabricated to screen the effect of 3D scaffold modulus on encapsulated osteoblasts . Arrays of salt-leached macro-porous scaffolds were prepared to measure osteoblast response to polymer blend composition . In other work, gradient and array library formats were compared for assessing osteoblast response to the mass fraction of amorphous calcium phosphate included in 3D composite salt-leached scaffolds . Finally, the effect of different extracellular matrix proteins on embryonic stem cell differentiation was studied using combinatorial hydrogel scaffold libraries .
In the current work, we aimed to develop an approach for fabricating gas-foamed scaffold gradients that can be used for combinatorial screening in 3D. Previously, we developed a two-syringe pump approach for fabricating salt-leached scaffold gradients [14,1820]. However, gas-foamed scaffolds have several advantages over salt-leached scaffolds. Gas-foamed scaffolds use gas bubbles to create porous polymer scaffolds . The gas-foaming process yields scaffolds with pores that are better connected than those in salt-leached scaffolds and gas-foamed scaffolds also have stronger mechanical properties . Salt-leaching also leaves a polymer skin on scaffolds that can prevent cells from
J. Funct. Biomater. 2012, 3
penetrating the scaffold interior while the gas-foaming process yields a scaffold with uniform pore distribution and no skin . Gas-foamed scaffolds support adhesion, proliferation and differentiation of osteoblasts to yield bone-like tissues [23,24].
A two-syringe pump approach (Figure 1) [18,19] was adapted to fabricate gas-foamed scaffold gradients. In order to demonstrate the feasibility of this approach, blends of two degradable tyrosine polycarbonates, poly(desaminotyrosyl-tyrosine ethyl ester carbonate) (pDTEc) and poly(desaminotyrosyl-tyrosine octyl ester carbonate) (pDTOc), were used to fabricate gas-foamed scaffold libraries. Tyrosine polycarbonates are being advanced for use in implantable biomedical devices such as hernia repair meshes, cardiovascular stents and bone tissue engineering scaffolds [25,26]. pDTEc and pDTOc have the same backbone but different side chains (Figure 2). These different side chains cause differences in the polymer properties including water contact angle (71 for pDTEc and 91 for pDTOc), glass transition temperature (99 C for pDTEc and 53 C for pDTOc), mechanics [pDTEc is brittle (4% elongation at break), while pDTOc is ductile (400% elongation at break)], degradation (pDTEc degrades faster) and biological response [14,27,28]. These differences in properties affect protein adsorption and cell responses such as cell spreading, adhesion and proliferation [27,28].
Figure 1. (a) Schematic representation of the combinatorial platform used to fabricate the gradient gas-foamed scaffold libraries. Solutions of pDTEc and pDTOc dispensed from programmed syringe pumps were mixed through a static mixer and deposited onto a trough of sieved NH4HCO3 crystals (250 m to 425 m); (b) Photograph of a Teflon rig supporting three gas-foamed gradient scaffolds in a large Petri dish. Each gradient is 75 mm long, 8 mm wide and 3 mm deep. A metal wire runs the length of each scaffold gradient enabling them to be suspended in the Petri dish for cell culture experiments.
2. Experimental Section
2.1. Fabrication of Gas-Foamed Gradient Scaffolds
Poly(desaminotyrosyl-tyrosine ethyl ester carbonate) (pDTEc, relative molecular mass 183,000 g/mol) and poly(desaminotyrosyl-tyrosine octyl ester carbonate) (pDTOc, relative molecular
J. Funct. Biomater. 2012, 3
mass 117,000 g/mol) were synthesized as described  and solutions of each were made in dioxane (0.1 g/mL). A two-syringe pump system [18,19] was used to fabricate gas-foamed scaffold gradients (Figure 1). Briefly, the pDTEc and pDTOc polymer solutions were loaded into syringes and placed on opposing syringe pumps. pDTEc solution (1 mL) was loaded on the left syringe pump and 2.5 mL of pDTOc solution was loaded on the right pump. The pumps were programmed for a run of 72 s such that the flow rate of the left pump (pDTEc) decreased linearly from 0.5 mL/min to zero while the flow rate of the right pump (pDTOc) increased linearly from zero to 0.5 mL/min. The two solution streams were mixed using a stainless steel static mixer (internal diameter 3.3 mm; catalog # EW-04669-54, Cole-Parmer) which mixes the polymer solutions by cutting and folding them as they flow through a series of helices. This process created effluent at a constant rate of 0.5 mL/min which changed linearly in composition from pDTEc to pDTOc as it eluted from the static mixer.
Figure 2. (a) Chemical structure of poly(desaminotyrosyl-tyrosine ethyl ester carbonate) (pDTEc) and poly(desaminotyrosyl-tyrosine octyl ester carbonate) (pDTOc); (b) FTIR spectra for pDTEc and pDTOc after baseline deduction and normalization to maximum absorbance.
Note: Peaks at 2,927 cm1 and 1,508 cm1 were chosen as the analytical and reference peak, re